Rougieux, Fiacre, E., Grant, Nicholas, E., Barugkin, Chug, Macdonald, Daniel and
Murphy, John D.. (2015) Influence of annealing and bulk hydrogenation on
lifetime-limiting defects in nitrogen-doped floating zone silicon. IEEE Journal of Photovoltaics, 5
(2). pp. 495-498.
Permanent WRAP url:
Copyright and reuse:
The Warwick Research Archive Portal (WRAP) makes this work of researchers of the
University of Warwick available open access under the following conditions.
This article is made available under the Creative Commons Attribution 3.0 (CC BY 3.0)
license and may be reused according to the conditions of the license. For more details
A note on versions:
The version presented in WRAP is the published version, or, version of record, and may
be cited as it appears here.
Influence of Annealing and Bulk Hydrogenation on
Lifetime-Limiting Defects in Nitrogen-Doped
Floating Zone Silicon
Fiacre E. Rougieux, Member, IEEE, Nicholas E. Grant, Chog Barugkin, Daniel Macdonald, Fellow, IEEE,
and John D. Murphy
Abstract—A recombination active defect is found in as-grown high-purity floating zone n-type silicon wafers containing grown-in nitrogen. In order to identify the properties of the defect, injection-dependent minority carrier lifetime measurements, secondary ion mass spectroscopy measurements, and photoluminescence lifetime imaging are performed. The lateral recombination center distribu-tion varies greatly in a radially symmetric way, while the nitrogen concentration remains constant. The defect is shown to be deac-tivated through high temperature annealing and hydrogenation. We suggest that a nitrogen-intrinsic point defect complex may be responsible for the observed recombination.
Index Terms—Floating zone, minority carrier lifetime, nitrogen, silicon.
THE presence of interstitial oxygen has been shown to neg-atively affect the minority carrier lifetime in silicon de-vices either through the boron–oxygen defect , , thermal donors , , other grown-in defects  or as a consequence of high temperature processing –. Hence, there is a grow-ing interest in the photovoltaic community in usgrow-ing oxygen-lean growth methods, such as the floating-zone (FZ) method to pro-duce wafers for high-efficiency silicon solar cells. However, relatively high concentrations of nitrogen are commonly mea-sured in silicon grown from the FZ method with typical nitrogen concentrations above1×1014 cm−3and up to the solubility of
∼4.5×1015 cm−3 from the atmosphere in which the crystals are grown . Nitrogen is well known to mitigate the impact of extended defects –. For instance, it effectively sup-presses the formation of vacancy and interstitial aggregates in FZ crystals ,  (by reacting with vacancies and silicon in-terstitials via the reactions N2+V→N2V and N2V+I→N2) . Nitrogen also pins dislocations , thus improving
me-Manuscript received August 26, 2014; revised October 20, 2014; accepted October 24, 2014. Date of publication December 19, 2014; date of current version February 18, 2015. This work was supported by the Australian Research Council, the Australian Renewable Energy Agency and the Engineering and Physical Sciences Research Council. The work of J. D. Murphy was supported by an Engineering and Physical Sciences Research Council First under Grant EP/J01768X/2.
F. E. Rougieux, N. E. Grant, C. Barugkin, and D. Macdonald are with the Research School of Engineering, College of Engineering and Computer Sci-ence, Australian National University, Canberra ACT 0200, Australia (e-mail: firstname.lastname@example.org; email@example.com; chog.barugkin@anu. edu.au; firstname.lastname@example.org).
J. D. Murphy is with the School of Engineering, University of Warwick, Coventry CV4 7AL, U.K. (e-mail: email@example.com).
Color versions of one or more of the figures in this paper are available online at http://ieeexplore.ieee.org.
Digital Object Identifier 10.1109/JPHOTOV.2014.2367912
chanical stability at high temperatures. Despite its many bene-fits, nitrogen also forms electrically active defects situated near the conduction band in FZ silicon . Upon subsequent an-nealing, these defects disappear and deeper defects are created –. The carrier lifetime (and hence solar cell efficiency) will potentially be affected by the presence of nitrogen-related defects. Unfortunately, very little data regarding the influence of nitrogen-related defects on the minority carrier lifetime have been published to date .
In this paper, we measure the minority carrier lifetime in nitrogen-doped FZ silicon and nitrogen-lean Cz silicon. While the lifetime is initially lower in the nitrogen-doped wafers, we show that it improves after high temperature annealing to values similar to the nitrogen-lean wafers. Through photoluminescence (PL) imaging, we show that the defect distribution may be re-lated to the vacancy distribution because of the radial symmetry observed. Finally, we demonstrate that the defect(s) can be par-tially hydrogenated using a hydrogen rich silicon nitride.
The samples used in this study were cut from two 100-mm di-ameter phosphorus-doped n-type silicon ingots. The first wafer of resistivity 1.5Ω·cm and thickness 250μm was from a control Cz ingot with no or very low nitrogen concentration. Three other wafers of resistivity 1.5Ω·cm and thickness 215μm were from a FZ ingot grown under both argon and nitrogen ambient. The nitrogen concentration in the nitrogen-doped wafers was mea-sured by secondary ion mass spectrometry (SIMS) performed by Evans Analytical Group. The detection limit was5×1013cm−3 and three measurements were made in each location.
One nitrogen-doped FZ wafer was RCA cleaned and an-nealed at 1000 °C for 1 h under nitrogen ambient. Following the high temperature anneal, the nitrogen-doped FZ wafer was etched in 5 wt% HF to remove any SiO2 film. All wafers were then RCA cleaned. One (nonannealed) nitrogen-doped FZ wafer was used to study the effect of hydrogenation on the defect density and was coated with plasma-enhanced chemical vapor-deposited (PECVD) silicon nitride (SiNX:H at 235°C for 1 h). The other wafers were coated with atomic-layer-deposited (ALD) aluminum oxide (Al2O3:H) deposited at 200°C and sub-sequently activated at 400°C in forming gas for 30 min, in order to activate the surface passivation.
Effective lifetime measurements were performed using the transient photoconductance method . The lifetime
496 IEEE JOURNAL OF PHOTOVOLTAICS, VOL. 5, NO. 2, MARCH 2015
Fig. 1. (a) Injection dependence of the measured lifetime for nitrogen-lean n-type Cz silicon and FZ nitrogen-doped n-type silicon. (b) Injection dependence of the measured lifetime: before and after annealing at 1000°C for 1 h. The intrinsic lifetime limit  is plotted as a solid line on both graphs.
measurements were obtained with a Sinton WCT120 system, where the sensing area has a diameter of 4 cm. PL lifetime im-ages were obtained using a BT Imaging LIS-R1 system . For PL imaging, the lifetime was measured at low injection, where the lifetime is less injection dependent. Considering the excel-lent passivation quality, the effective defect concentration was calculated asN∗t = 1/τresidual = 1/τm easured−1/τintrinsic us-ing a recent intrinsic (Auger and band-band) lifetime parame-terization .
A. Influence of Nitrogen on the Minority Carrier Lifetime in as-Grown and Thermally Processed Silicon
Fig. 1(a) shows the measured injection dependence of the lifetime of the Cz wafer and the nitrogen-doped FZ wafer. The lifetime of the nitrogen-doped sample in the as-grown state is clearly limited by recombination active defects. The oxygen and carbon concentrations are expected to be significantly lower than1×1016 cm−3 and are below the detection limit of
stan-dard SIMS or Fourier transform infrared spectroscopy measure-ments. However, nitrogen concentrations of 4.6×1014 cm−3 were measured with SIMS in this nitrogen-doped wafer. Hence, it is possible that nitrogen plays a role in the observed recombi-nation active defect.
Fig. 1(b) shows the measured-injection dependent lifetime of the samples before and after annealing at 1000°C for 1 h (pas-sivated with Al2O3:H). The lifetime increases from 450μs to above 3 ms. Provided the recombination active defect observed is nitrogen related, this change in lifetime could correspond to the defect transformation observed by others in nitrogen-doped FZ silicon using deep level transient spectroscopy (DLTS) . Such behavior was observed in as-grown FZ silicon doped with nitrogen, but not in nitrogen-free FZ silicon ,  and was shown to disappear after 900°C anneal for 3 h . Its con-centration was also found to scale with the N concon-centration and to be in concentrations of7×1011−8×1011 cm−3 (for total nitrogen concentrations of1.9×1015 cm−3) .
The majority nitrogen species in silicon is the split interstitial dimer . The recombination activity in our samples is not con-sistent with recombination through a defect with a∼1014cm−3 concentration, as this would require the defect to have unphys-ically small capture cross sections. Our study is, thus, further evidence for the nitrogen dimer not having any states in the gap . Therefore, our defect, if nitrogen related, is most likely a minority nitrogen-containing species.
B. Spatial Distribution of the Defect Density and Potential Composition of the Defect
Fig. 2. Low-injection PL image of the nitrogen-doped FZ silicon sample before annealing with (a) Al2O3:H passivation and (b) SiNX:H passivation. Lifetimes
are measured inμs. (c) Profile of the effective defect density is plotted across the wafer, and the SIMS nitrogen measurements at the two tested regions are also plotted.
Fig. 3. (a) Residual minority carrier lifetime as a function of the p/n ratio before and after annealing at 1000°C for 1 h and after the deposition of a hydrogen containing film SiNX:H. (b) Injection dependence of the measured lifetime before and after the deposition of a hydrogen containing film SiNX:H. The line on
(b) represents the intrinsic limit . The lifetime increases significantly after the hydrogenation procedure.
vacancies could constitute the observed recombination active defect.
C. One or Many Defect Species?
There have been many different complexes between vacancies and nitrogen identified previously (VXNY) . The question remains whether only one species is responsible for the observed low lifetime, or if a combination of different defects is respon-sible. Fig. 3(a) shows the measured injection dependence of the lifetime, corrected for intrinsic recombination, as a function of the ratio of total hole concentration (p) to the total electron con-centration (n). A linear behavior in such a plot would imply the existence of just one single-level defect . The absence of a single linear trend over the whole injection range suggests that at least two defects (or perhaps one defect with two levels) are responsible for the observed reduced lifetime . The defect pa-rameters cannot be determined in this case, as this requires the availability of samples with significantly different doping levels.
D. Hydrogenation of the Defect
Regardless of their structure, the observed defect(s) has(have) the potential to significantly degrade the performance of high-efficiency n-type silicon solar cells, especially rear-junction so-lar cells, which are most sensitive to the carrier lifetime in the wafer bulk. However, such cells are likely to incorporate a de-position step of silicon nitride, amorphous silicon or aluminum oxide, potentially leading to partial hydrogenation of the bulk. Such hydrogenation could potentially alter the recombination activity of the nitrogen-vacancy centers.
498 IEEE JOURNAL OF PHOTOVOLTAICS, VOL. 5, NO. 2, MARCH 2015
shows the injection dependence of the lifetime for samples pas-sivated with these two films. Note that photoconductance-based lifetime measurements (averaged over an area of 4 cm) are af-fected by spatial lifetime nonuniformities; thus, the shape of the injection dependent lifetime curve may be slightly inaccurate. In any case, the samples which have been passivated with PECVD SiNX:H have significantly higher lifetimes than the samples passivated with ALD Al2O3:H. Measurement on control wafers shows similar passivation for SiNX:H and Al2O3:H; hence, the improved lifetime in the nitrogen-doped wafers is not due to differences in surface passivation. Instead, our results suggest hydrogen may be able to passivate a significant fraction of the recombination active defect(s).
In conclusion, we show that one defect or multiple de-fects limit(s) the lifetime in highly pure nitrogen-doped n-type floating zone silicon wafers. A very low bulk level of nitro-gen (∼5×1014 cm−3) is suggested to give rise to a minority nitrogen-containing species, which reduces the lifetime from 4.8 ms to below 450μs at an injection of1×1015 cm−3. By measuring the spatial distribution of the defect, our initial study suggests the most likely candidate for the observed recombi-nation active defect is a vacancy and nitrogen-related defect VXNY. We demonstrate that the defect can be removed during high temperature processing of standard silicon solar cells, con-sistent with previous studies on nitrogen-related defects using DLTS. For low-temperature-processed silicon solar cells, such as heterojunction solar cells, the defect will still be present in the finished solar cell. In order to mitigate the impact of the defect, one can either perform a high temperature annealing prior to processing or a hydrogenation procedure.
 A. Richter, S. W. Glunz, F. Werner, J. Schmidt, and A. Cuevas, “Improved quantitative description of Auger recombination in crystalline silicon,”
Phys. Rev. B, vol. 86, art. no. 165202, 2012.
 J. Schmidt and K. Bothe, “Structure and transformation of the metastable boron- and oxygen-related defect center in crystalline silicon,” Phys. Rev.
B, vol. 69, art. no. 024107, 2004.
 K. Bothe and J. Schmidt, “Electronically activated boron-oxygen-related recombination centers in crystalline silicon,” J. Appl. Phys., vol. 99, art. no. 013701, 2006.
 Y. Hu, H. Schon, O. Nielsen, E. J. Ovrelid, and L. Arnberg, “Investigating minority carrier trapping in n-type Cz silicon by transient photoconduc-tance measurements,” J. Appl. Phys., vol. 111, art. no. 053101, 2012.  Y. Hu, H. Schon, E. J. Ovrelid, O. Nielsen, and L. Arnberg, “Investigating
thermal donors in n-type Cz silicon with carrier density imaging,” AIP
Adv., vol. 2, art. no. 032169, 2012.
 F. E. Rougieux, N. E. Grant, and D. Macdonald, “Thermal deactivation of lifetime-limiting grown-in point defects in n-type Czochralski silicon wafers,” Physica Status Solidi—Rapid Res. Lett., vol. 7, pp. 616–618, 2013.
 K. Bothe, R. J. Falster, and J. D. Murphy, “Room temperature sub-bandgap photoluminescence from silicon containing oxide precipitates,”
Appl. Phys. Lett., vol. 101, art. no. 032107, 2012.
 J. D. Murphy, K. Bothe, M. Olmo, V. V. Voronkov, and R. J. Falster, “The effect of oxide precipitates on minority carrier lifetime in p-type silicon,”
J. Appl. Phys., vol. 110, art. no. 053713, 2011.
 J. D. Murphy, K. Bothe, R. Krain, V. V. Voronkov, and R. J. Falster, “Parameterisation of injection-dependent lifetime measurements in semiconductors in terms of Shockley-Read-Hall statistics:
An application to oxide precipitates in silicon,” J. Appl. Phys., vol. 111, art. no. 113709, 2012.
 J. Haunschild, I. E. Reis, J. Geilker, and S. Rein, “Detecting efficiency-limiting defects in Czochralski-grown silicon wafers in solar cell produc-tion using photoluminescence imaging,” Physica Status Solidi—Rapid
Res. Lett., vol. 5, pp. 199–201, 2011.
 H. Angelskar, R. Sondena, M. S. Wiig, and E. S. Marstein, “Characteriza-tion of oxida“Characteriza-tion-induced stacking fault rings in Cz silicon: Photolumines-cence imaging and visual inspection after wright etch,” Energy Procedia, vol. 27, pp. 160–166, 2012.
 Y. Yatsurugi, N. Akiyama, Y. Endo, and T. Nozaki, “Concentration, solu-bility, and equilibrium distribution coefficient of nitrogen and oxygen in semiconductor silicon,” J. Electrochem. Soc., vol. 120, pp. 975–979, 1973.  W. v. Ammon, P. Dreier, W. Hensel, U. Lambert, and L. K¨oster, “Influ-ence of oxygen and nitrogen on point defect aggregation in silicon single crystals,” Mater. Sci. Eng. B, vol. 36, pp. 33–41, 1996.
 T. Abe and H. Takeno, “Dynamic behavior of intrinsic point defects in Fz and Cz silicon crystals,” MRS Online Proc. Library, vol. 262, art. no. 3, 1992.
 C. R. Alpass, J. D. Murphy, R. J. Falster, and P. R. Wilshaw, “Nitrogen diffusion and interaction with dislocations in single-crystal silicon,” J.
Appl. Phys., vol. 105, art. no. 013519, 2009.
 W. von Ammon, R. H¨olzl, J. Virbulis, E. Dornberger, R. Schmolke, and D. Gr¨af, “The impact of nitrogen on the defect aggregation in silicon,” J.
Cryst. Growth, vol. 226, pp. 19–30, 2001.
 K. Nauka, M. S. Goorsky, H. C. Gatos, and J. Lagowski, “Nitrogen-related deep electron traps in float zone silicon,” Appl. Phys. Lett., vol. 47, pp. 1341–1343, 1985.
 Y. Tokumaru, H. Okushi, T. Masui, and T. Abe, “Deep levels associated with nitrogen in silicon,” Jpn. J. Appl. Phys., vol. 21, art. no. L443, 1982.  T. Abe, H. Harada, N. Ozawa, and K. Adomi, “Deep level generation-annihilation in nitrogen doped FZ crystals,” MRS Online Proc. Library, vol. 59, art. no. 537, 1985.
 K. Kakumoto and Y. Takano, “Deep level induced by diffused N2 and
vacancy complex in Si,” in Proc. 2nd Int. Symp. Adv. Sci. Technol. Silicon
Mater., 1996, art. no. 437.
 J. D. Murphy, C. R. Alpass, A. Giannattasio, S. Senkader, D. Emiroglu, J. H. Evans-Freeman, R. J. Falster, and P. R. Wilshaw, “Nitrogen-doped sil-icon: Mechanical, transport and electrical properties,” ECS Trans., vol. 3, pp. 239–253, Oct. 2006.
 W. V. Ammon and P. Dreier, “Silicon bulk technology for power devices,” in Proc. Int. Symp. Power Semicond. Devices, 1988, pp. 134–140.  R. A. Sinton and A. Cuevas, “Contactless determination of current–
voltage characteristics and minority-carrier lifetimes in semiconductors from quasi-steady-state photoconductance data,” Appl. Phys. Lett., vol. 69, pp. 2510–2512, 1996.
 T. Trupke, R. A. Bardos, M. C. Schubert, and W. Warta, “Photolumi-nescence imaging of silicon wafers,” Appl. Phys. Lett., vol. 89, art. no. 044107, 2006.
 R. Jones, S. ¨Oberg, F. Berg Rasmussen, and B. Bech Nielsen, “Identifica-tion of the dominant nitrogen defect in silicon,” Phys. Rev. Lett., vol. 72, pp. 1882–1885, 1994.
 J. P. Goss, I. Hahn, R. Jones, P. R. Briddon, and S. ¨Oberg, “Vibrational modes and electronic properties of nitrogen defects in silicon,” Phys. Rev.
B, vol. 67, art. no. 045206, 2003.
 V. V. Voronkov and R. Falster, “Grown-in microdefects, residual vacancies and oxygen precipitation bands in Czochralski silicon,” J. Cryst. Growth, vol. 204, pp. 462–474, 1999.
 V. V. Voronkov and R. Falster, “Intrinsic point defects and impurities in silicon crystal growth,” J. Electrochem. Soc., vol. 149, pp. G167–G174, 2002.
 A. Focsa, A. Slaoui, H. Charifi, J. P. Stoquert, and S. Roques, “Surface passivation at low temperature of p- and n-type silicon wafers using a dou-ble layer a-Si:H/SiNx:H,” Mater. Sci. Eng. B, vol. 159–160, pp. 242–247, 2009.
 G. Dingemans, M. C. M. van de Sanden, and W. M. M. Kessels, “Influence of the deposition temperature on the c-si surface passivation by Al2O3 films synthesized by ALD and PECVD,” Electrochem. Solid-State Lett., vol. 13, pp. H76–H79, 2010.
 B. Sopori, M. I. Symko, R. Reedy, K. Jones, and R. Matson, “Mecha-nism(s) of hydrogen diffusion in silicon solar cells during forming gas anneal,” in Proc. IEEE 26th Photovoltaic Spec. Conf., 1997, pp. 25–30.